A fixture to apply compressive loads to composite specimens during an impact event was used to assess the effect of prestresses on the compressionafter ...
NASATHIIIST9
, A/
THE
EFFECTS OF COMPRESSIVE COMPRESSIONAFTERIMPACT CARBON/EPOXY
Y'. ', 
PRELOADS ON THE STRENGTH OF
Alan T. Nettles NASA,
Marshall Space Flight Mail Zone Eit33 Huntsville,
Center
AL 35812
ABSTRACT A fixture
to apply
used to assess
compressive
the effect
loads to composite
of prestresses
specimens
during an impact
on the compressionafterimpact
event was
(CA[)
strength
of
16 ply quasiisotropic carbon/epoxy test coupons. Advanced design of experiments techniques were used to evaluate a range of prestresses and impact energies on two material systems, between
T300/934 and IM7/85517. An instrumented drop tower supplied impact energies 1 and 9 Joules for the T300/934 material and between 4 and 16 Joules for the
IM7/85517
material.
287 MPa.
Results
prestresses
KEY
The prestress
showed
some
values varied between
change
Composites,
Impact
Resistance,
1.
A vast amount materials.
of research
In virtually
has been
all studies
stresses during the impact stress during an accidental have
in CA] strength that could be attributed
its bottom
INTRODUCTION
performed
conducted,
in the area of impact the composite
skin mostly
service/maintenance. in a compressive
prestresses on composite materials undergoing NASA workshop on impact damage tolerance the purpose
Little Awa
of this research
of composite
Awa
damage
specimen
to composite
was under
is to assess
The wing, being a cantilever state. The need
of assessing
no external a state of the bottom
of
beam, will
the effects
of
foreign object impact was identified at a of composite materials held in 1991 (1). Thus
the effects
of compressive
preloads
on the impact
specimens.
experimental data exists on impact of preloaded composite specimens. Rhodes and have presented data that contain information on this subject (2,3). Rhodes concluded
that the residual stressed
Testing Equipment
event. In actual practice a composite may be under foreign object impact, for example a worker hitting
skin with a tool during
behavior
to the
on the specimens.
WORDS:
a wing
a low of 5.7 MPa and a high of
compressive
state is slightly came
to a similar
strength
of specimens
lower than those impacted conclusion
but showed
impacted
while
when no external
in a compressive stress
that at high impact energies,
was applied. the preload had a
"//;t ....
smallerdetrimentaleffect the tensile samples
prestresses
on CA/strength
needed
of a variety
to cause
of materials
than at lower impact energies.
catastrophic
including
Park (4) examined
failure for a given impact
carbon fiber reinforced
epoxy.
energy
in
Two tup sizes
were used to represent an impact from a blunt and a sharp impactor. "Impact maps" or the line of catastrophic failure on an impact energy versus prestress chart were plotted for various
materials.
Little data on residual
Sun (5) and Dabyns nofceable by tensile When
(6) have analytically
changes
frequencies
in impact
or compressive
analyzed
parameters
of the composite
performing
strength of surviving
plates.
this problem
are those
Maximum
specimens
was given.
and found that the most
dealing with changes
in the fundamental
load of impact was not effected
Very much
preloads.
experimental
work,
especially
of a destructive
nature,
it can become
time
consuming and expensive to examine a number of variables by holding all but one constant and examining the response of the material to that one variable that is changing. In addition, two variables interact with one another, this would not be noticed in onevariableatatime testing.
Thus
be a very
utilizing
efficient
2.1 Design
advanced
design
and effective
of Experiments
to conduct
laboratory
2.
EXPERIMENTAL
Two multivariable
was used to evaluate
to examine
way
effects of compressive prestresses load of impact of two carbon/epoxy design
of experiments
and impact materials.
T300/934
more than one variable
if can
tests.
test matrices
were
used to assess
the
energy on the CA[ strength and maximum A full factorial three level two parameter
carbon/epoxy,
and a central
composite
five level two
parameter design was used to evaluate IM7/85517 carbon/toughened epoxy. The test matrices are shown in tables 1 and 2. Data were analyzed with a designed experiments software
package
(BBN/Catalyst).
Run Number 1 2
5.7
5.0
3
5.7
9.0
4
60.3
1.0
5
60.3
5.0
6
60.3
9.0
7
115
1.0
8
115
5.0
115
9.0
9
_ Table
The output data consists the response
Impact Energy 1.0
Prestress (MPa) 5.7
variable
1. Parameter
of one constant
(either
maximum
settings
and five coefficients. load of impact
independent variables (prestress and impact The five coefficients relate the linear effects of their quadratic of the independent
effects
on the constant
variables
material. The constant
or CAI strength)
when
is the value
of
the two
energy) are at their centermost or mean values. of the two parameters, their interaction and each
value.
must be normalized
to a high value of+l. For example, = 1, 60.3 MPa = medium = 0 and
for T300/934
(Joules)
In order to use these between
a low of1
in table 1, the values of prestress 115 MPa = high = +1. The values
coefficients,
the values
to a mean
of zero, up
become 5.7 MPa = low of the impact energy
become 1.0 Joules = low  1, 5.0 Joules = medium = 0 and 9.0 Joules = high  +1. The normalized values are dimensionless. The effect of the five coe_cients are found by multiplying adding
each coefficient
by the normalized
this value to the constant.
independent
variables'
6.0
3
144
4
144
6.0
5
201
4.3
6
201
15.7
7
115
I0.0
8
287
10.0
9
201
I0.0
settings
for IM7/85517
material.
of Experiments Suppose that the constant for a given set of runs is found to be 5000 Newtons and the coefficients are:
N = 1000 N Energy Interaction
Quadratic
Impact
=  100 N
= 250 N Energy
= 750 N
that when the prestress
Joules, the resulting
maximum
values,
+1. The corresponding Prestress (MPa) 5.7
is set at 60.3 MPa and the impact energy
load of impact
will be 5000 N. To normalize
set the low values to 1, the medium actual values to normalized Normalized
in table 3. (J)
Normalized 1
2.0
33.0
.5
3.0
.5
46.7
.25
4.0
.25
60.3
0
5.0
74
+.25
6.0
0 +.25
88
+.5
7.0
+.5
101
+.75
g.o
+.75
115
+1
9.0
+I
of the two independent
variables.
3. Actual
and corresponding
normalized
values
and
values to 0 and the high values to
values is given Impact Energy I.O
1
is 5.0
the prestress
.75
19.4
Table
(Joules)
14.0
Prestress
energy
Impact Energy 14.0
258
= 500
and then
value for the given
2
Quadratic
impact
it represents
Prestress (MPa) 258
2.1.1 Example of Design for the T300/934 material
This indicates
response
1
Table 2. Parameter
Impact Energy Prestress/Impact
variable(s)
values.
Run Number
Prestress
independent
This will yield the predicted
.75
Now suppose the value of the maximum load of impact is to be predicted for a prestress of 101 MPa and 3.0 J of impact energy. The normalized values are now, prestress = +.75 and Impact
Response
energy
=  .5. The predictive
equation
is:
= 5000N 500 N(+.75) +1000 N(.5) 100 N(+.75)(.5) 250 N (+.75) 2 750 N (.5) 2 = 3834
N
The genera/equation
can be written as:
Response
4 (Prestress
 Constant
Coefficient)fNormalized
Impact
Coet_cient)(Normalized Energy)
+ (Interaction
Prestress)
4 (Impact
Energy
Coefficient)(Normalized
Prestress)(Normalized Impact Energy) + (Quadratic Prestress Coeffident)(Normalized Prestress) 2 + (Quadratic Impact Energy Coefficient)(NolT,n, alizod Impact Energy) 2 i
2.2 Test Coupons The specimens used were 16 ply [0,+45,90,4512S quasiisotropic a nominal ply thickness of.127 mm. The specimen dimensions were 178 mm !ongby
with 76mm,
wide with a gage length of 102 mm leaving 38 mm on each end for tabs. The compressive preloads
were introduced
the apparatus
into the specimens
used to apply
Specimen
the prestress
Support Plate (Removable)
using
an end loading
to the specimens
Pressure Platen
technique.
Figure
1 shows
during impact.
Load Cell
_==
Front Wall
Back Wail
===
3m
4 Ram Moves
This
_r51
mm
"l_ lib..
508 mm Figure In order gages
to ensure
were placed
a uniform
1. Compression
prestress
on the specimen
was present
as shown
preload device. at the area to be impacted,
in figure 2.
n
Back
Figure
Face
2. Placement
Impacted of strain
Face
gages and dimensions
of specimens.
three
strain
The strain gages were monitored as the prestress was applied and ifa deviation of more than 10% occurred between any of the three gages, the test was halted and another specimen was used. A deviation in the gages usually indicated that the specimen ends were not cut to close enough
tolerances
to evenly
2.3 Compression
Preload
distribute Device
the stress being applied to the ends of the specimen. A fixture
consisting
hydraulic
ram was used to apply the appropriate
manually
driven via a hand pump
other and apply a compressive
basically
prdoads
before
of two steel plates and a impact.
such that the two, parallel plates would
load to the specimen
loca_d
between
The ram was approach
each
the tWO plates
(see_
_
•figure 1). A load cell was placed between the ram and one of the steel plates to record the applied preload. The specimen rested on a steel block with a 63 mm diameter hole cut through it. A removable specimen support plate with a matching 63 mm circular cutout was placed on top of the specimen and clamped lightly to the steel block so as to sandwich most of the gage
length
of the specimen
2.4 CompressionAfterImpact
providing
an antibuckling
Testing
support.
After the specimens
were impacted
while
subjected to the various preloads, they were tested for residual compression strength. shear loading fixture with supporting faceplates was used to test the relatively thin specimens.
A more detailed
description
of this test method
3. RESULTS
3.1 Load/Strain taken at various uniform
AND
can be found elsewhere
A (7).
DISCUSSION
During Preload The load/strain data from the three strain gages were increments of loading for all of the specimens tested. This assured that a
external
stress field was being
plot of the load/strain
applied at the area to be impacted.
data for T300/934
specimen
Figure
# 6.
300O •
Gage
I
y = 9.4353
+ 0.53777x
+
Gage
2
y = 9.5990
+ 0.55021x
_, j
200O
I tooo
!
0
1000
I
!
2000
3000
Load
Figure
3. Preload/strain

4000
5000
(ibs)
data for T300/934
specimen
# 6.
3 shows
a
This specimen example
demonstrated
of a specimen
strain gages
a very uniform
strain field at the area to be impacted.
that had to be discarded
exceeds
20%.
2000
•
Gage
1750 _
+
Gage 2
Y = 1.5820
+ 0.47382x
1500 ]
e
Gage 3
y ffi 92.986
+ 0.46882x
el
]
I
y :
 152.22
An
is given in figure 4 where the deviation
in the
+ 0.63585x
sI
1250 1
z.,
o tl
0
500
1000
1500
Load
Figure
4. Preload/strain
2000
2500
(ibs)
data for a discarded
T300/934
specimen.
3.2 Impact Testing The maximum impact load, as well as several other parameters, were recorded after each impact. A Dynatup 730 data acquisition system was used with an instrumented
tup of 12.7 mm diameter.
After each impact, the specimen
was removed
from
the preload device and the visual damage was noted and recorded. No catastrophic failures occurred for the T300/934 material. A catastrophic break is an event where the specimen fails in compression with zero residual The maximum
due to the combination
loads for the T300/934
Prestress
specimens
Impact Energy
(MPa)
are given (J)
in table 4.
Maximum
Load of Impact
5.7
1.0
1129
5.7
5.0
3054
5.7
9.0
3772
4
60.3
1.0
5
60.3
5.0
2503
6
60.3
9.0
3267
7
115
1.0
925
8
115
5.0
2630
9
115
9.0
2928
1 3
#
Table As theorized "softening"
4. Maximumim
by Sun and Chen effect
a specimen
strength.
impact
Run #
of preload and impact thus yielding
_act load for the T300/934
(4), an initial compressive
on the laminate
stiffness
1075
i
stress
specimens. will give rise to a
and thus lower maximum
impact
loads for a given
impactlevel.
This seems to be the case for the T300/934 material since the highest loads occurred consistently at the lowest prestress levels. A more detailed analysis data will he presented The maximum
later in this paper.
load of impact
Run #
impact of these
Prestress
for the IM7/85517 (MPa)
specimens
Impact Energy
are given
(J)
in table 5. Load of Impact
Maximum
(IT) 14.0
3056
258
6.0
2844
144
14.0
3249
4
144
6.0
3168
5
201
4.3
2584
6
201
15.7
3570
7
115
10.0
3392
8
287
10.0
2948
9
201
10.0
3418
1
258
2 3
Table 5. Maximum These
data also show a "softening"
preload.
impact load for IM7/85517 effect
This will also be examined
3.3 Residual on impact,
Compression
Strength
for the T300/934
material axe given Run #
material
stiffness
due to a compressive
in further detail later in this paper. For thespecimens
the compressionaRerimpact
The results
on the laminate
specimens.
(CAI) are given
that did not failcatastrophically
strength was measured
as described
in table 6 and the results for the IM7/85517
in table 7. Prestress(MPa) 5.7
(CA/) Strength(MPa) 372
Impact Ener_/(J) 1.0
5.7
5.0
291
5.7
9.0
293
60.3
1.0
395
5
60.3
5.0
288
6
60.3
9.0
297
7
115
1.0
446
8
115
5.0
294
9
I15
9.0
276
Table #
Run
6. Compressionafterimpact Prestress (MPa) 258
strength data for T300/934 Impact Ener_
(J)
(CA/)
specimens.
Strength
2
258
14.0 6.0
3
144
14.0
308
4
144
6.0
315
5
201
4.3
328
6
201
15.7
261
7
115
10.0
299
8 9
287 201
10.0 10.0
Catastrophic 290
Table
earlier.
7. Compressionafterim
tact strength
(MPa)
Catastrophic Impact 302
data for IM7/85517
Impact
specimens.
All of the specimens 3.4 Analysis
tested for residual
of Data
strength
The data for maximum
broke at the impacted
area.
load of impact and for residual compressive
strength were evaluated with an advanced design of experiments methodology. The T300/934 material was evaluated using a full factorial experiment while the IM7/85517 material was evaluated with a central composite fractional factorial experiment 3.4.1 Maximum software
Load
program
of lmpact;
that would
T300/934
generate
The data from table 4 were entered
quantitative
values for the influence
into a
of first  and
secondorder (quadratic) effects of both preioad and impact energy, as well as any interaction these two variables may have with one another The following coefficients
_ were
generated: Constant
= 2646
Prestress
= 245 N
Impact Energy Prestress/Impact
N
= 1140 N Energy Interaction
Quadratic
Prestress
Quadratic
Impact Energy
= 125 N
A good way to examine maximum
=  160 N
= 546 N these
load of impact
coefficients
on the vertical
is to create a "surface (z) axis versus preload
response"
on one horizontal
impact energy on the other horizontal (3') axis. Figure 5 is a surface maximum load of impact versus impact energy and preload.
,0
plot, or a plot of
response
(x) axis and
plot of
115
60.3
5.7'x
Prestress (Mpa) Figure
5. Maximum
The prestress
has little influence
variable
is seen when
laminate
"softening"
yield much
load of impact
higher
on the maximum
the prestress impact
impact
energy
loads
preloads.
and prestress:
T300/934.
load of impact. A slight increase
is at the lower end of settings
due to compressive maximum
versus
As expected,
with a leveling
which
demonstrates
the higher
offoccurring
of this
impact
the
energies
at the high end when
fiber breakage needed 3.4.2
begins
to perforate Maximum
plot shown
to develop
in the specimen
and the impact
load comes
closer to that
the specimen.
Load
oflmpact;
IM7/85517
The data from table 5 will give the response
in figure 6.
o
Figure
6. Maximum
load of impact
The following coefficients IM7/85517 material: Constant
= 3418
Prestress
= 216 N
Impact Energy Prestress/Impact
Prestress
Quadratic
Impact
This material The largest At the other
were generated
impact
energy and prestress:
for the maximum
IM7/85517.
impact load response
for the
N
= 316 N Energy
Quadratic
versus
Interaction
= 0 N
= 308 N Energy
= 409 N
has a maximum impact
impact
loads occur
extremes
when
the impact
load that is als o dependent the prestress
load decreases.
on the amount
is near the medium This trend holds
of prestress.
or 201 MPa setting.
for all values
of _[npact
energy (indicating no interaction). is to be expected and the maximum
As the prestress is increased, a "softening" of the laminate impact load will decrease for a given impact energy. As
the prestress obvious.
for the decrease
A direct
decreases,
comparison
IM7/85517 were more
of the maximum
material severe
the reason
is not practically
for the toughened
in maximum
impact
impact load data for the T300/934 feasible IM7/855
since the prestress I7.
load is not as
material
and impact
and the
energy
levels
3.4.3 Compression.AfterImpact of compressionafterimpact The coefficients are: Constant
7"300/'934 Figure 7 shows the response surface energy and prestress for the T300/934 material.
 291 MPa
Prestress Impact
Strength; versus impact
= 10.0 MPa Energy
= 57.8 MPa
Prestress/Impact
Energy
Quadratic
Prestress
Quadratic
Impact
Interaction
= 22.8 MPa
= O MPa Energy
= 55.5 MPa
O _"J
Figure The CA/strength also dependent
I
7. CAI strength is heavily
versus
dependent
on the amount
impact
upon
of prestress
energy and prestress:
the impact
energy
in the specimen.
used
T300/934. (as expected)
The dependence
but is
is linear
and
interacts with the amount of impact energy that is being used. At the low end of impact energy, the CAI strength increases with increasing prestress, and at the larger impact energies,
the CA/strength
to the "softening" effective stiffness maximum
decreases
slightly
with increasing
preload.
This can be attributed
effect mentioned earlier where a compressive prestress of the laminate thus producing a more damage resistant
load of impact
plot (figure
5) shows
this effect where
will decrease the material. The
the more highly
prestressed
specimens show a small decrease in maximum impact load. The change in this trend at the high end of impact energies can be attributed to the specimen reaching its perforation level and in this case the "sottening"
seen at lower impact
energies
will become
negligible
due to
the extremely hard hits the specimen is undergoing. The slight decrease in CA/strength at higher preloads is due to the specimens reaching their catastrophic breaking point which indicates that the preload can further damage the specimen while the impact damage is being induced 3.4.3
into the specimen.
CompressionAfterImpact
surface of compressionafterimpact material. The coefficients are:
Strength; versus
IM785517
Figure
8 shows
impact energy and prestress
the response for the IM7/85517
Constant=
297 MPa = 93.0 MPa
Prestress Impact
Energy
= 50.5
MPa
Prestress/Impact Energy Interaction Quadratic Prestress = 70.9 MPa Quadratic
Impact
Energy
= 73.8
MPa
= 0 MPa
Oq
g','ll IIII
tllllk
144
_'_
p
2ol restress
Figure
The extreme energy
8. CAI strength
(Alpa) versus
impact energy and prestress:
drop in CAI strength with increasing
is due to the catastrophic
break implies
zero residual
preload combined
IM7/85517.
with increasing
impact
breaks that occurred on runs # 1 and 8. (A catastrophic
strength).
The linear dependence
of CAI strength
on impact
energy is unusual and is probably due to the strong impact energy/prestress interaction coupled with a tough resin system. Toughened resin composites have shown different trends in loss of CAI strength material
with increasing
was prestressed
impact energy (8). In addition,
and impacted
at much more severe
levels
than the T300/934
material and the level of impact at which a sudden drop in CAI strength included.
4.
the IM7/85517 occurs
is not
CONCLUSION
For a brittle carbon/epoxy system such as T300/934, layedup as 16 ply (0,+45,90,45)2S coupons and tested at impact energies up to 9 J, the effects of compressi_,e prestresses up to 115 MPa on maximum impact
energy.
load of impact were found to be small compared
At the impact level where the maximum
the preload (9 J), a 27 % increase
in maximum
prestresses seen
carbon/epoxy
have a slightly
in this variable
tested
smaller
at much more severe
effect
of by
impact load is seen as the preload decreases
from its highest level to its lowest level. Given that the impact energies not at a level severe enough to cause catastrophic failure, this difference For a toughened
to the effect
impact load was most affected
on the maximum
from the 258 MPa prestress
impact impact
and prestresses were may be significant.
energies load.
and preloads,
A 19 % increase
to the 221 MPa prestress
values
the is
at the
impact energy that is most affected by the preioads which is the lowest level. This smaller difference could be from the fact that even at the lower end of prestresses used with this
.t
material, significant "softening" ofthe material being impacted still occurred. 7 material was tested at much higher prestresses than the T300/934 material. The compressionafterimpact
(CA/)
strength
of the T300/934
material
The IM7/8551
was affected
by the
amount of prestress, especially at the extreme values of impact energy used. At the lowest level (1.0 J), a 18 % increase in CA.[ strength is seen as the preioad increases from its lowest to highest
values.
At the highest
(9.0 J) level, a 8.6 % decrease
is seen in the CA[ strength
the coupons as the preload increased from its lowest to highest values. The "softening" effect of the compressive preload can account for the behavior in the CAI strength at_e lower impact energies.
At the higher
level such that the "softening" impact
impact energies,
effect
to helping
i _,
was hit at a high enough the specimen
have better
resistance.
The CA/strength
of the IM7/85517
specimens
especially
at the higher
occurring
on runs # 1 and 8. A 13 % decrease
impact
the specimen
did not contribute
of_
energy
end ofirnpact
was severely
energies
(6.0 J) as the prestress
by the prestress,
used. This was due to catastrophic
failures
in CA[ strength was seen at the lower end of
was increased
higher value of 258 MPa. At the higher
effected
from its lower value of 144 MPa to the
impact energy
(14.0 J) the decrease
was 98 %.
5. SUMMARY
When
a composite
effect
will occur that increases
specimen
of impact and increasing impacted
at severe
is impacted
while
the specimens
the CA/strength.
levels
under a compressive
damage resistance, However,
near the breaking
prestress,
a "softening"
reducing the maximum
when the specimen
point of the specimen,
load
is prestressed
the opposite
trend
and occurs
and the specimen can fail catastrophically resulting in zero residual compressive strength, if the specimen survives, the CAI strength may decrease due to the preload, and any "softening"
of the specimen
by the compressive
prestress is negated
by the high level of
impact.
6. REFERENCES
1.
NASA
2.
(1991). M.D. Rhodes,
CP 10075,
Workshop
J. G. Williams
on Impact Damage and J. H. Starnes,
to Composites, Jr., polymer
Hampton,
Composites.
VA, 2, (1), 36
(1981). 3.
V.S.
4. 5.
ASTM, Philadelphia, 1986, pp.196, N. Park, _ C400/019 (1990). C.T. Sun and J. K. Chert, J.CM...1_
6.
A.L.
Dobyns,
7.
A.T.
Nettles
8.
(1991). R.L. Dempsey (1990).
Avva,
J. R. Vala and M. Jeyasseelan
J.,/MAA
in J. M. Whitney,
ed., ASTM
STP 893,
206. 490 (1985).
J.. 19. 642 (1981).
and A. J. Hodge,
SAMPE
and R. E. Horton,
International
SAMPE
Technical
International
Conference.
Symposium.
_
23. 177 1292
or
¸